|Year : 2022 | Volume
| Issue : 2 | Page : 160-170
|Flexural strength of CAD/CAM denture base materials: Systematic review and meta-analysis of in-vitro studies
Reem Abualsaud, Mohammed M Gad
Department of Substitutive Dental Sciences, College of Dentistry, Imam Abdulrahman Bin Faisal University, P. O. Box 1982, Dammam, Kingdom of Saudi Arabia
|Date of Submission||04-Nov-2021|
|Date of Decision||11-Dec-2021|
|Date of Acceptance||22-Dec-2021|
|Date of Web Publication||08-Apr-2022|
Dr. Reem Abualsaud
Department of Substitutive Dental Sciences, College of Dentistry, Imam Abdulrahman Bin Faisal University, P. O. Box 1982, Dammam 31441.
Kingdom of Saudi Arabia
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Introduction: Digital complete dentures fabrication techniques are expanding. This study aimed to review flexural strength (FS) of milled and 3D-printed denture base materials to answer the study question: is FS of computer-aided designing/computer-aided manufacturing (CAD/CAM) denture base comparable to conventional heat-polymerized materials?Materials and Methods: Search was done within different databases for articles published between January 2010 and June 2021 using specific keywords. Articles of in-vitro studies in English language with methods following International Standards Organization standardization/ADA specifications for flexural testing of conventional and CAD/CAM (milled or printed) polymethyl methacrylate (PMMA) materials were included. Results: Out of the 61 studies, 9 were processed for data extraction and only 7 underwent meta-analysis. Two, six, and one study showed high, moderate, and low risk of bias, respectively. Random-effects model was used for analysis and resulted in the average FS of 120.61 MPa [95% confidence interval (CI): 109.81−131.41] and 92.16 MPa (CI: 75.12−109.19) for CAD/CAM milled and heat-polymerized PMMA, respectively. Conclusion: Subtractive CAD/CAM technique of denture fabrication showed satisfactory FS values, whereas additive CAD/CAM method was comparable to conventional heat-polymerized technique with lower value, requiring further investigations and improvement. The clinical use of milled denture bases is an acceptable substitution to heat-polymerized PMMA, making the denture fabrication an easier and faster process.
Keywords: 3D-printed denture base, CAD/CAM denture base, flexural strength, PMMA
|How to cite this article:|
Abualsaud R, Gad MM. Flexural strength of CAD/CAM denture base materials: Systematic review and meta-analysis of in-vitro studies. J Int Soc Prevent Communit Dent 2022;12:160-70
|How to cite this URL:|
Abualsaud R, Gad MM. Flexural strength of CAD/CAM denture base materials: Systematic review and meta-analysis of in-vitro studies. J Int Soc Prevent Communit Dent [serial online] 2022 [cited 2022 May 19];12:160-70. Available from: https://www.jispcd.org/text.asp?2022/12/2/160/342728
| Introduction|| |
Scientists are on the path to find a technique that will eliminate or reduce the downsides seen with conventional denture fabrication technique that has been used for more than eight decades and improve the mechanical, physical, and optical properties of the polymethyl methacrylate (PMMA) material. This improvement maybe brought up by the introduction of computer-aided designing/computer-aided manufacturing (CAD/CAM) technology. In this technique, the obtained information from the patient is converted into digital data using specific computerized software., Based on this information, the denture is designed digitally and saved in STL (Standard Triangle Language) format upon which the denture is produced in a subtractive (milling) or additive (3D-printing) technique.,,,,
Conventional method of fabrication involves lengthy procedures of technique-sensitive material manipulation, complex and lengthy procedures of denture waxing, investing, dewaxing, packing, and polymerization of heat-polymerized PMMA that undergoes a degree of polymerization shrinkage resulting in slight inaccuracy of final denture.,, In comparison, the digital process can accomplish similar results with less number of clinical visits, allow visualization of residual ridge and denture to be made from different aspects, permit digital record keeping, and improve patient satisfaction. Additionally, CAD/CAM milled dentures provide better adaptation and retention of the denture.,[12-19] Milled dentures are produced by subtractive trimming from readymade pre-polymerized pucks of resin that were fabricated under strict conditions of elevated temperature and pressure to produce highly dense material. This process reduces further polymerization during denture fabrication and allows the production of dentures with adequate mechanical properties in thinner sections. This permits better speech and higher patient comfort.,,,,
Digitally fabricated dentures are produced by either additive (3D-printing) or subtractive (milling) methods. Milling of acrylic dentures is widely spreading, but 3D-printing affords a variety of advantages over milling, such as being economical and enabling concurrent manufacturing of many products. In contrast, the accuracy of dentures made by subtractive manufacturing is reliant on the milling tools number, size, and configuration, whereas additively manufactured dentures reproducibility is developing with the technology.
Since the use of 3D-printing technology is still in its initial stages and is continuously evolving, there is a deficit of reported data regarding mechanical properties of these materials. Only few studies reported the FS of 3D-printed resin being lower than other types of PMMA. Others reported that pure 3D-printed PMMA had lower FS value that improved upon reinforcement with fillers.
Regardless of the advantages associated with CAD/CAM technology, scientific evidences regarding mechanical properties of CAD/CAM fabricated prostheses are lacking. Hence, this review was prepared to evaluate and compare the FS of milled and 3D-printed PMMA denture base material to heat-polymerized acrylic resin.
| Materials and Methods|| |
This systematic review was prepared inline with the Preferred Reporting Items for Systematic Reviews and Meta-analyses (PRISMA) statement and the Patient or Population, Intervention, Control or Comparison, and Outcome (PICOS) approach. The PICOS question was: is the flexural strength (FS) of CAD/CAM (milled or 3D-printed) denture base materials comparable with the conventional heat-polymerized denture base materials? Where the participants groups were complete denture base materials, and intervention groups are CAD/CAM denture bases, in comparison to conventional heat-polymerized denture bases with the outcome of included studies being the flexural strength. To answer this question, studies complying to the following inclusion criteria were included in the analysis.
Inclusion criteria comprised full-length in-vitro studies, written in English language, and comparing between FS of CAD/CAM and heat-polymerized denture base materials using ISO standardization/ADA specifications for testing. Articles not meeting these criteria were excluded. Search was done using PubMed, Google Scholar, EM-BASE, Scopus, and Web of Science databases for articles published between January 2010 and June 2021 with the last search date being July 7, 2021. The search keywords were CAD/CAM denture base, PMMA, flexural strength, CAD/CAM, computer-aided, computer-assisted, digital, 3D-printing, milled, complete denture/s, and a combination of two or more of them.
The review was done in three steps. First, two independent reviewers evaluated the titles of all acquired articles according to the inclusion criteria, and discrepancies were resolved by discussion. Secondly, abstracts of the selected titles were screened and those of interest were marked for full-text analysis. At the third step, selected full-text articles were examined and the data were tabulated in a template. Among the extracted data are the author’s names, year or publication, materials used, brand names and manufacturers, specimen dimensions, sample size, storage medium, results, and outcome.
The authors modified the Cochrane risk of bias tool to fit the objective of the study. The risk of bias of included studies (n=9) was evaluated by two authors using an adaptation of the methods applied in a previous systematic review. During this process, parameters were reported as yes (when mentioned/available) or no (when absent).
JASP 0.14.1 was used for statistical analysis. In the meta-analysis, presence of heterogeneity in the data was checked first to select the proper model for further analysis. Random-effects model was employed in cases in which heterogeneity in data was found, whereas fixed-effects model was used otherwise. Visual inspection of forest plots and χ2 tests were used to test the presence of heterogeneity. Possibility of publication bias was evaluated by Egger’s test and visual inspection of funnel plots.
| Results|| |
The initial search of the databases provided (n=61) studies [Figure 1]. Titles irrelevant to the research question, duplicate titles, and publications in languages other than English were excluded This process yielded 25 studies that were further scrutinized to ensure meeting inclusion criteria. At the end, nine studies,,[27-33] were included for data extraction and analysis. [Table 1] presents a summary of extracted data.
[Figure 2] summarizes the risk of bias for the included studies. Out of the nine included studies, six,,[28-31] showed medium risk, two, showed high risk of bias, and one showed low risk of bias. The risks of bias reported were mainly due to missing information regarding sample size calculation and blinding of examiners.
Out of the nine final included articles, eight,[27-33] compared FS of milled denture base with heat-polymerized denture base, whereas only one study compared milled, 3D-printed, and heat-polymerized denture bases. The nine included studies followed ISO standardization/ADA specification regarding specimen dimensions and testing for three-point bending test. For the denture base materials used, a wide range of pre-polymerized CAD/CAM discs, 3D-printing material, and heat-polymerized PMMA were used [Table 1]. Seven studies,[27-31], were included in the meta-analysis, whereas two studies did not either mention the means or presented the results in a chart making data extraction difficult.
Included in the meta-analysis of milled denture bases are seven studies with 10 total treatment groups, one of which was eliminated for being an outlier. For heat-polymerized method, seven studies were included with height total observations. Visual inspection of forest plots and χ2 tests for both groups (milled and heat-polymerized) revealed the presence of heterogeneity (I2 >75%, P-value<0.001) [Figures 3] and . Hence, the random-effects model was used. The average FS for milled PMMA was 120.61 MPa [95% confidence interval (CI): 109.81−131.41] and for heat-polymerized 92.69 MPa (95% CI: 73.58−111.79). The shape of the funnel plots for both groups (milled and heat-polymerized) was not clear to draw any conclusion about the presence of publication bias. Therefore, Egger’s test was used and the results were insignificant (P-value=0.55, 0.976), respectively, which suggests the absence of publication bias.
According to the meta-analysis results, milled materials showed higher FS value when compared with heat-polymerized. In between milled materials, three studies,, milled specimens to desired dimensions using milling machines, whereas the other six studies,,[27-29], cut the pre-polymerized acrylic resin blocks using diamond saw with no variation in results averages. One study assessed the FS of 3D-printed resin, and the results were presented as minimum and maximum values with no mention of the mean. However, the 3D-printed material recorded the lowest FS value between all tested PMMA materials.
| Discussion|| |
High FS of resin base material is a prime factor for denture durability and prevention of failures under load., During denture life, it is exposed to repeated cycles of masticatory forces. This repeated action may lead to denture cracking, fracture, and failure. This failure is potentiated in the presence of poor fit, improper design, or notches. In such situations, the fracture of the denture happens after the maximum flexure fatigue is exceeded. The FS test is defined as maximum stress experienced by a material at its point of yielding and is considered a collective reflection of the material’s tensile, shear, and compressive strengths. The three-point bending test has been adopted by the ISO as the recommended test for FS of polymers with acceptable clinical value set to be not less than 65 MPa (ISO 1567).
Resins available to fabricate denture bases are polymerized using a variety of ways including heat, chemical, visible light, and microwave energy. Although the process is rapid, it is never complete, and a percentage of free monomer is still detected after polymerization. In addition, heat-polymerized dentures may contain porosities due to uncontrolled heating, improper mixing, monomer evaporation, or inadequate pressure during polymerization. Additionally, bases may have crazing as a result of water incorporation during polymerization or warpage due to incorporated stresses., Volumetric and linear shrinkages are inherent to heat-polymerized resin; therefore, occlusal adjustments are normally required after de-flasking. Similarly, carving of a post-dam groove in the cast is partially indicated to compensate for the shrinkage occurring after polymerization that may cause the lift-off the palatal section of the denture.
As CAD/CAM PMMA pucks are manufactured in extremely controlled environment, they are produced in a highly dense state with minimal shrinkage, porosity, or free monomers., The milling process utilizes pre-polymerized pucks, which eliminates processing errors. The literature has reported better attributes of milled denture bases, including mechanical and biological properties, in addition to good surface characteristics.
FS, among others, may indicate the degree of polymerization of the resin, whereas lower degree of conversion will result in inferior mechanical properties including FS. Consequently, higher FS values reported for milled specimens can be linked to higher degrees of conversion. Therefore, one can assume that the equipment used to pre-polymerize pucks is capable of polymerizing the acrylic resin to higher degree than conventional heat-polymerized.
According to the meta-analysis, milled denture base resins showed high FS (120.61 MPa) compared with heat-polymerized PMMA (92.16 MPa). The difference was mainly attributed to milling the denture out of a completely pre-polymerized PMMA puck., When CAD/CAM pucks are produced, longer chains of polymer are created, which means higher rate of conversion and minimal residual monomer reducing its plasticizing effect and improving the FS, minimal porosity, less internal stress and flaws, minimal intermolecular distances, and higher material resistance.,,,,,,
The conventional processing technique induces linear shrinkage (0.45−0.9%), whereas digital processing virtually eliminates further shrinkage. Murakami et al. recommended processing heat-polymerized PMMA at high pressure to increase molecular weight of polymer matrix and to decrease residual monomer and internal voids.,
The reported results of FS of milled denture base material varied.,,[27-33] Al-Dharrab and Pacquet et al. reported superiority of heat-polymerized PMMA than milled PMMA. Srinivasan et al., Aguirre et al., and Hada et al. all concluded that milled PMMA had better mechanical properties than heat-polymerized PMMA. Perea-Lowery et al. showed a significant variation in mechanical properties of the tested materials with heat-polymerized PMMA showing the highest FS value. However, the performance of all resins was satisfactory. These findings suggest the applicability of using heat-polymerized PMMA for denture fabrication as CAD/CAM resins did not show better mechanical properties. Al-Dwairi et al. exhibited in a previous study better FS, impact strength, and flexural modulus of milled PMMA when compared with heat-polymerized resin. At another level, Steinmassl et al. failed to detect the source of the residual monomer or report significant difference between different PMMA types.
Prpić et al. reported the highest FS with milled PMMA followed by heat-polymerized then lastly 3D-printed PMMA. This study was the only one included in this review that evaluated FS of 3D-printed PMMA. Although the 3D-printed material used had the lowest FS value, it met the ISO recommendation for FS (65 MPa) and is suggested as an option for the fabrication of denture bases. The variation in the reported values could be associated with material’s structure. The downside of the 3D-printed acrylic is the low double-bond conversion in comparison with other types of acrylic resins, which in turn could affect the mechanical properties. Due to the limited number of studies, additional research is recommended to reach conclusions regarding mechanical properties of 3D-printed denture base PMMA and to evaluate its applicability for the fabrication of dentures with properties comparable to those of milled or heat-polymerized PMMA.
Photopolymerization of solvent-free resins offers economical and countless uses in dentistry. For optimal clinical performance, the resins should possess high curing rate, storage stability, low viscosity, and adequate biological properties and results in a final product with high mechanical and physical properties., Total conversion of the monomer is not guaranteed after polymerization, and systemic side effects may occur as a result of exposure to residual monomer or degradation products. To correlate this to clinical situation, structurally poor acrylic resin may cause cytotoxic effects to oral tissues and impede protein synthesis of epithelial cells.
The degree of double bond conversion during polymerization is an important indicator of physical and mechanical properties of the resulting resin. It refers to the amount of double bonds between carbon atoms that are transformed into single bonds; i.e., monomer is converted to polymer., The result of incomplete conversion means that free monomer is suspended to the end product with possible leach-out and tissue irritation. For 3D-printed materials, no definitive conclusion exists to correlate between conversion rate and biological effects. Therefore, new formulations must be carefully used due to the variation in constituents, structure, or functionality. One should take into consideration that the extent of polymerization is dependent on multiple factors such as the composition including the concentration of photoinitiator, specimen geometry, and curing environment.
Looking at the acrylic specimens from a different perspective, only two studies used scanning electron microscopy for analysis of fractured surface or to detect surface characteristics. Generally, brittle fractures will show compact and smooth appearance of fracture site, whereas rough and irregular surface suggests intermediate (brittle to ductile) fracture modes., The fractographic appearance of milled and heat-polymerized materials predominantly showed brittle fractures. Confined zones of intermediate fractures were seen with milled materials. Arslan et al. found that conventional PMMA exhibited more pores and surface irregularities than milled PMMA.
Steinmassl et al. were the first to report variation of physical properties between different brands of milled PMMA after reporting different densities of dentures made from four brands. These results might be linked to variations in the initial processing of PMMA to produce the pre-polymerized pucks.
Clinically, higher mechanical strength of milled PMMA may allow for thinner denture bases/palatal plates that comprise more natural speech and feel and higher degree of patient comfort and satisfaction, although evidence is still lacking till the moment., If future studies confirm the longevity of the milled PMMA strength after cyclic fatigue, they would be considered valuable alternatives in cases presenting with high functional loads, cases with repeated denture fractures, overdentures without metal reinforcement, implant-supported overdentures in cases with limited inter-arch space, or hollowed and lightweight maxillo-facial prostheses for oncology patients.
Finally, the authors would like to report the limitations of this study such as the low number of included studies; only one of the included studies did thermocycling and another one evaluated 3D-printed denture bases. Therefore, further studies evaluating the FS and other mechanical properties of milled and 3D-printed PMMA in oral environment-simulated conditions are necessary. Fractography analysis of fracture sites to determine the behavior of material failure is also recommended.
| Conclusions|| |
Based on the reviewed literature, most of the studies reported satisfactory FS of milled specimens in comparison to heat-polymerized PMMA. 3D-printing of denture bases was comparable to conventional heat-polymerized PMMA, but showed lower FS value necessitating further investigations. Until further research and advancement in material composition and property of 3D-printed resin, milled and heat-polymerized PMMA resins remain the materials of choice to fabricate denture bases with high flexural strength.
The authors would like to thank Mr. Soban Khan for his assistance with statistical analysis.
Financial support and sponsorship
The author(s) received no financial aid for the research, authorship, or publication of this study.
Conflicts of interest
The authors have no conflicts of interests to declare.
Both the authors contributed to study design, data acquisition and interpretation, and manuscript writing and finalization.
Ethical policy and institutional review board statement
Patient declaration of consent
Data availability statement
The data supporting the findings of this study are available within the manuscript and its supplementary materials.
| References|| |
Paulino MR, Alves LR, Gurgel BC, Calderon PS Simplified versus traditional techniques for complete denture fabrication: A systematic review. J Prosthet Dent 2015;113:12-6.
Al-Dwairi ZN, Tahboub KY, Baba NZ, Goodacre CJ, Özcan M A comparison of the surface properties of CAD/CAM and conventional polymethylmethacrylate (PMMA). J Prosthodont 2019;28:452-7.
Infante L, Yilmaz B, McGlumphy E, Finger I Fabricating complete dentures with CAD/CAM technology. J Prosthet Dent 2014;111:351-5.
AlHelal A, AlRumaih HS, Kattadiyil MT, Baba NZ, Goodacre CJ Comparison of retention between maxillary milled and conventional denture bases: A clinical study. J Prosthet Dent 2017;117:233-8.
Kattadiyil MT, Goodacre CJ, Baba NZ CAD/CAM complete dentures: A review of two commercial fabrication systems. J Calif Dent Assoc 2013;41:407-16.
Bilgin MS, Erdem A, Aglarci OS, Dilber E Fabricating complete dentures with CAD/CAM and RP technologies. J Prosthodont 2015;24:576-9.
Wimmer T, Gallus K, Eichberger M, Stawarczyk B Complete denture fabrication supported by CAD/CAM. J Prosthet Dent 2016;115:541-6.
Bidra AS, Taylor TD, Agar JR Computer-aided technology for fabricating complete dentures: Systematic review of historical background, current status, and future perspectives. J Prosthet Dent 2013;109:361-6.
Bilgin MS, Baytaroğlu EN, Erdem A, Dilber E A review of computer-aided design/computer-aided manufacture techniques for removable denture fabrication. Eur J Dent 2016;10:286-91.
Abduo J, Lyons K, Bennamoun M Trends in computer-aided manufacturing in prosthodontics: A review of the available streams. Int J Dent 2014;2014:783948.
Lim SR, Lee JS Three dimensional deformation of dry-stored complete denture base at room temperature. J Adv Prosthodont 2016;8:296-303.
Steinmassl PA, Wiedemair V, Huck C, Klaunzer F, Steinmassl O, Grunert I, et al
. Do CAD/CAM dentures really release less monomer than conventional dentures? Clin Oral Investig 2017;21:1697-705.
Srinivasan M, Gjengedal H, Cattani-Lorente M, Moussa M, Durual S, Schimmel M, et al
. CAD/CAM milled complete removable dental prostheses: An in vitro
evaluation of biocompatibility, mechanical properties, and surface roughness. Dent Mater J 2018;37:526-33.
Kattadiyil MT, Jekki R, Goodacre CJ, Baba NZ Comparison of treatment outcomes in digital and conventional complete removable dental prosthesis fabrications in a predoctoral setting. J Prosthet Dent 2015;114:818-25.
Goodacre BJ, Goodacre CJ, Baba NZ, Kattadiyil MT Comparison of denture base adaptation between CAD-CAM and conventional fabrication techniques. J Prosthet Dent 2016;116:249-56.
Srinivasan M, Cantin Y, Mehl A, Gjengedal H, Müller F, Schimmel M CAD/CAM milled removable complete dentures: An in vitro
evaluation of trueness. Clin Oral Investig 2017;21:2007-19.
Steinmassl O, Dumfahrt H, Grunert I, Steinmassl PA CAD/CAM produces dentures with improved fit. Clin Oral Investig 2018;22:2829-35.
Kattadiyil MT, AlHelal A, Goodacre BJ Clinical complications and quality assessments with computer-engineered complete dentures: A systematic review. J Prosthet Dent 2017;117:721-8.
Kattadiyil MT, AlHelal A An update on computer-engineered complete dentures: A systematic review on clinical outcomes. J Prosthet Dent 2017;117:478-85.
Koike T, Ishizaki K, Ogami K, Ueda T, Sakurai K Influence of anterior palatal coverage on perception and retention in complete dentures. J Prosthet Dent 2011;105:272-9.
Berman B 3-D printing: The new industrial revolution. Bus Horiz 2012;55:155-62.
Bosch G, Ender A, Mehl A A 3-dimensional accuracy analysis of chairside CAD/CAM milling processes. J Prosthet Dent 2014;112:1425-31.
Prpić V, Schauperl Z, Ćatić A, Dulčić N, Čimić S Comparison of mechanical properties of 3d-printed, CAD/CAM, and conventional denture base materials. J Prosthodont 2020;29:524-8.
Chen SG, Yang J, Jia YG, Lu B, Ren L TiO2 and PEEK reinforced 3D printing PMMA composite resin for dental denture base applications. Nanomaterials (Basel) 2019;9:1049.
Goujat A, Abouelleil H, Colon P, Jeannin C, Pradelle N, Seux D, et al
. Marginal and internal fit of CAD-CAM inlay/onlay restorations: A systematic review of in vitro
studies. J Prosthet Dent 2019;121:590-7.e3.
Faggion CM Jr. Guidelines for reporting pre-clinical in vitro
studies on dental materials. J Evid Based Dent Pract 2012;12:182-9.
Al-Dharrab A The residual monomer content and mechanical properties of CAD/CAM resins used in the fabrication of complete dentures as compared to heat cured resins. Electron Phys 2017;9:4766-72.
Arslan M, Murat S, Alp G, Zaimoglu A Evaluation of flexural strength and surface properties of prepolymerized CAD/CAM PMMA-based polymers used for digital 3d complete dentures. Int J Comput Dent 2018;21:31-40.
Pacquet W, Benoit A, Hatège-Kimana C, Wulfman C Mechanical properties of CAD/CAM denture base resins. Int J Prosthodont 2019;32:104-6.
Aguirre BC, Chen JH, Kontogiorgos ED, Murchison DF, Nagy WW Flexural strength of denture base acrylic resins processed by conventional and CAD-CAM methods. J Prosthet Dent 2020;123:641-6.
Al-Dwairi ZN, Tahboub KY, Baba NZ, Goodacre CJ A comparison of the flexural and impact strengths and flexural modulus of CAD/CAM and conventional heat-cured polymethyl methacrylate (PMMA). J Prosthodont 2020;29:341-9.
Perea-Lowery L, Minja IK, Lassila L, Ramakrishnaiah R, Vallittu PK Assessment of CAD-CAM polymers for digitally fabricated complete dentures. J Prosthet Dent 2021;125:175-81.
Hada T, Kanazawa M, Iwaki M, Katheng A, Minakuchi S Comparison of mechanical properties of PMMA disks for digitally designed dentures. Polymers 2021;13:1745.
Zappini G, Kammann A, Wachter W Comparison of fracture tests of denture base materials. J Prosthet Dent 2003;90:578-85.
Kelly E Fatigue failure in denture base polymers. J Prosthet Dent 1969;21:257-66.
Jagger DC, Harrison A, Jandt KD The reinforcement of dentures. J Oral Rehabil 1999;26:185-94.
Abdulwahhab SS High-impact strength acrylic denture base material processed by autoclave. J Prosthodont Res 2013;57:288-93.
International Organization for Standardization (ISO). Dentistry—base polymers—Part 1: Denture base polymers. ISO 20795-1:2013. Available from: https://www.iso.org/standard/62277.html.
Karci M, Demir N, Yazman S Evaluation of flexural strength of different denture base materials reinforced with different nanoparticles. J Prosthodont 2019;28:572-9.
Wong DM, Cheng LY, Chow TW, Clark RK Effect of processing method on the dimensional accuracy and water sorption of acrylic resin dentures. J Prosthet Dent 1999;81:300-4.
Sanders JL, Levin B, Reitz PV Comparison of the adaptation of acrylic resin cured by microwave energy and conventional water bath. Quintessence Int 1991;22:181-6.
Gharechahi J, Asadzadeh N, Shahabian F, Gharechahi M Flexural strength of acrylic resin denture bases processed by two different methods. J Dent Res Dent Clin Dent Prospects 2014;8:148-52.
Steinmassl O, Offermanns V, Stockl W, Dumfahrt H, Grunert I, Steinmassl PA In vitro
analysis of the fracture resistance of CAD/CAM denture base resins. Materials (Basel) 2018;11:401.
Nguyen JF, Migonney V, Ruse ND, Sadoun M Resin composite blocks via high-pressure high-temperature polymerization. Dent Mater 2012;28:529-34.
Kawara M, Komiyama O, Kimoto S, Kobayashi N, Kobayashi K, Nemoto K Distortion behavior of heat-activated acrylic denture-base resin in conventional and long, low-temperature processing methods. J Dent Res 1998;77:1446-53.
Arita T, Kayama Y, Ohno K, Tsujii Y, Fukuda T High-pressure atom transfer radical polymerization of methyl methacrylate for well-defined ultrahigh molecular-weight polymers. Polymer 2008;49:2426-9.
Murakami N, Wakabayashi N, Matsushima R, Kishida A, Igarashi Y Effect of high-pressure polymerization on mechanical properties of PMMA denture base resin. J Mech Behav Biomed Mater 2013;20:98-104.
Alifui-Segbaya F, Bowman J, White AR, George R, Fidan I Characterization of the double bond conversion of acrylic resins for 3d printing of dental prostheses. Compend Contin Educ Dent 2019;40:e7-11.
Li J, Cui Y, Qin K, Yu J, Guo C, Yang J, et al
. Synthesis and properties of a low-viscosity UV-curable oligomer for three-dimensional printing. Polym Bull 2016;73:571-85.
Vitale A, Cabral JT Frontal conversion and uniformity in 3D printing by photopolymerisation. Materials (Basel) 2016;9:760.
Kim SH, Watts DC Degree of conversion of bis-acrylic based provisional crown and fixed partial denture materials. J Korean Acad Prosthodont 2008;46:639-43.
Stansbury JW, Dickens SH Determination of double bond conversion in dental resins by near infrared spectroscopy. Dent Mater 2001;17:71-9.
Powers JM, Wataha JC Dental Materials. Foundations and Applications. 11th ed. Philadelphia, PA: Elsevier Health Sciences; 2017.
Sideridou I, Tserki V, Papanastasiou G Effect of chemical structure on degree of conversion in light-cured dimethacrylate-based dental resins. Biomaterials 2002;23:1819-29.
Alifui-Segbaya F, Bowman J, White AR, Varma S, Lieschke GJ, George R Toxicological assessment of additively manufactured methacrylates for medical devices in dentistry. Acta Biomater 2018;78:64-77.
Faot F, Costa MA, Del Bel Cury AA, Rodrigues Garcia RC Impact strength and fracture morphology of denture acrylic resins. J Prosthet Dent 2006;96:367-73.
Praveen B, Babaji HV, Prasanna BG, Rajalbandi SK, Shreeharsha TV, Prashant GM Comparison of impact strength and fracture morphology of different heat cure denture acrylic resins: An in vitro
study. J Int Oral Health 2014;6:12-6.
Lee HH, Lee CJ, Asaoka K Correlation in the mechanical properties of acrylic denture base resins. Dent Mater J 2012;31:157-64.
[Figure 1], [Figure 2], [Figure 3], [Figure 4]
| Article Access Statistics|
| Viewed||802 |
| Printed||18 |
| Emailed||0 |
| PDF Downloaded||132 |
| Comments ||[Add] |